# 2782 IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 60, ... 2782 IEEE TRANSACTIONS ON ELECTRON DEVICES,...

date post

16-Oct-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of 2782 IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 60, ... 2782 IEEE TRANSACTIONS ON ELECTRON DEVICES,...

2782 IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 60, NO. 9, SEPTEMBER 2013

Performance Analysis of Strained Monolayer MoS2 MOSFET

Amretashis Sengupta, Member, IEEE, Ram Krishna Ghosh, and Santanu Mahapatra, Senior Member, IEEE

Abstract— We present a computational study on the impact of tensile/compressive uniaxial (εxx) and biaxial (εxx = εyy) strain on monolayer MoS2, n-, and p-MOSFETs. The material properties like band structure, carrier effective mass, and the multiband Hamiltonian of the channel are evaluated using the density functional theory. Using these parameters, self-consistent Poisson–Schrödinger solution under the nonequilibrium Green’s function formalism is carried out to simulate the MOS device characteristics. 1.75% uniaxial tensile strain is found to provide a minor (6%) ON current improvement for the n-MOSFET, whereas same amount of biaxial tensile strain is found to considerably improve the p-MOSFET ON currents by 2–3 times. Compressive strain, however, degrades both n-MOS and p-MOS devices performance. It is also observed that the improvement in p-MOSFET can be attained only when the channel material becomes indirect gap in nature. We further study the perfor- mance degradation in the quasi-ballistic long-channel regime using a projected current method.

Index Terms— Density functional theory (DFT), MoS2, MOSFET, nonequilibrium Green’s function (NEGF), strain.

I. INTRODUCTION

AMONG the various classes of alternate channel mate-rials under research, the 2-D materials having nonzero bandgap in their sheet form like the transition metal dichalco- genides (MX2:M = Mo, W; X = S, Se, and Te) seem very promising for MOSFET applications. This is due to their better electrostatic integrity, optical transparency, mechanical flexibility, and the geometrical compatibility with the standard planar CMOS technology. Among such MX2 materials the performance of MoS2-based MOS transistor and logic have been successfully demonstrated experimentally [1], [2]. This has generated great interest in studying such nongraphene 2-D crystals for future MOSFET channel application [3]–[5].

The main challenge in such 2-D MoS2 FETs, so far has been to overcome the low carrier mobility of channel [1], [2]. For Si CMOS, strain engineering has long been used to enhance carrier mobility and improve drive currents and other

Manuscript received February 7, 2013; revised June 19, 2013; accepted July 12, 2013. Date of publication July 26, 2013; date of current version August 19, 2013. This work was supported in part by the Depart- ment of Science and Technology and Government of India under Grant SR/S3/EECE/0151/2012. The review of this paper was arranged by Editor A. Schenk.

The authors are with the NanoScale Device Research Laboratory, Department of Electronic Systems Engineering, Indian Institute of Sci- ence, Bangalore 560012, India (e-mail: amretashis@dese.iisc.ernet.in; ramki.phys@gmail.com; santanu@cedt.iisc.ernet.in).

Color versions of one or more of the figures in this paper are available online at http://ieeexplore.ieee.org.

Digital Object Identifier 10.1109/TED.2013.2273456

Fig. 1. Device schematic (not to scale) and diagram showing the applied uniaxial and biaxial tensile and compressive strains. We consider doped source and drains. K → � direction is taken as the transport direction.

device parameters [6]. Recent reports suggest that monolayer MoS2 and other MX2 also show alteration of material proper- ties like band structure and carrier effective masses under the influence of strain [7]–[10]. In addition, Ghorbani-Asl et. al. in [11] have shown the impact of strain on the conductance in MoS2 sheets. Hence, strain engineering in principle, could be used to improve the performance of MoS2. In this paper, we investigate the impact of tensile and compressive uniaxial (εxx) and biaxial (εxx = εyy) strain on the performance of monolayer MoS2, n-MOS, and p-MOS devices. In this paper, the material properties of 2-D (monolayer) MoS2, like band structure, carrier effective mass, and the multiband Hamiltonian of the channel, were evaluated using the density functional theory (DFT). Using these parameters, the MOS device output characteristics were simulated by solving the Poisson and the Schrödinger equations self-consistently for the system, under the nonequilibrium Green’s function (NEGF) formalism. The device simulation results show only a minor performance enhancement for the n-MOSFET under uniaxial tensile strain. On the other hand, the p-MOSFET performance is significantly improved by reducing the carrier effective mass by applying biaxial tensile strain.

II. METHODOLOGY

Fig. 1 shows the schematic device structure of the planar 2-D MoS2 FET considered for our research. We consider a monolayer MoS2 as the channel material, with channel length (LCh) of 10 nm. As shown in Fig. 1, the ten- sile and the compressive strains are considered applied in the two perpendicular directions x and y in the plane of the 2-D sheet. For uniaxial strain only εxx is applied whereas for

0018-9383 © 2013 IEEE

SENGUPTA et al.: PERFORMANCE ANALYSIS OF STRAINED MONOLAYER MoS2 MOSFET 2783

the biaxial case strain is applied in both x and y directions with εxx = εyy. The 2-D channel is placed over an SiO2/Si substrate. High-κ HfO2 of 2.5-nm thickness is chosen as the gate dielectric. We consider highly doped (1020 /cm3) n++ and p++ regions as the source/drain for the n-MOSFET and the p-MOSFET, respectively. Such doping concentrations allow for a very good alignment of the source/drain Fermi levels with the conduction band/valence band for the monolayer MoS2, n-, and p-MOSFETs [4], [5]. For our simulations, K → � direction (x direction in Fig. 1) is taken as the transport direction.

The first step, in this paper, is to evaluate the elec- tronic properties of the channel material (i.e., strained and unstrained monolayer MoS2 sheets). For this pur- pose, we employ DFT in QuantumWise Atomistix Tool Kit (ATK) [13]. We use a 16 × 16 × 1 Monkhorst- Pack k-grid [14], [15] and employ the localized den- sity approximation [15] exchange correlation function with the double-zeta polarized (DZP) basis [14]. We use Troullier– Martins type norm-conserving pseudopotential sets in ATK (NC-FHI[z = 6] DZP for Sulfur and NC-FHI[z = 6] DZP for Molybdenum). Relativistic corrections are included in the nonlinear core [13]. Using DFT, we simulate the band structure and the electron and the hole effective masses of the monolayer MoS2. The multiband 41 × 41 Hamiltonain matrix (H ) and the nonorthogonal overlap matrix (S) are extracted from ATK at the valence band maxima (VBmax) and the conduction band minima (CBmin) of the band structure, for various strained and relaxed conditions. As with applied strain, the nature of the bandgap of the monolayer changes from direct to indirect gap, we extract the Hamiltonians at the corresponding CBmin for the n-MOSFET, and at the corresponding VBmax for the p-MOSFET simulations.

Thereafter, we proceed to solve the Poisson and Schrödinger equations self-consistently for our MoS2 FET. The self- consistent solutions are carried out under the NEGF formalism [16], [17]. In our solver, we construct the Green’s function from the knowledge of the H and S matrices and the energy eigenvalue matrix E of the system along with the self- energy matrices �S and �D of the source and drain contacts, respectively. The Green’s function is then evaluated as [16] follows:

G(E) = [E S − H − �S − �D]−1. (1) From (1), parameters like the broadening matrices ℘S and

℘D and the spectral densities AS and AD are evaluated using the following relations:

℘S,D = i [�S,D − �+S,D]. (2) AS,D = G℘S,DG+. (3)

The density matrix [�] used to solve the Poisson equation is given by

[�] = ∫ ∞

−∞ d E

2π [A(Ek,x)] f0(Ek,x − η) (4)

where A(Ek,x) is the spectral density matrix, Ek,x is the energy of the conducting level, and η being the chemical potential

Fig. 2. Effect of uniaxial (εxx ) and biaxial (εxx = εyy ) tensile (+) and compressive (−) strain on the bandgap of the monolayer MoS2.

of the contacts. f0(.) is the Fermi function. The transmission matrix �(E) is calculated as follows:

�(E) = trace[AS℘D] = trace[AD℘S]. (5) Thus, giving out the ballistic drain current ID,Bal as [3]

follows:

ID,Bal = q h̄2

√ mtϕT h

2π3

∫ ∞ −∞

[ F−1/2

( ηS − Ek,x

ϕT h

)

−F−1/2 (

ηD−Ek,x ϕT h

) ] �(Ek,x )d E

(6)

mt being the carrier effective mass in the transverse direction, ϕTh is the thermal energy, Ek,x is the energy of the conducting level, F−1/2 is the Fermi integral of order −1/2. ηS and ηD are the chemical potentials of the source and drain, respectively. It is notable that the current calculated in (6) is purely ballistic in nature, which holds well for channels of short dimensions up to few tens of nanometers. However, for longer channel lengths the transmission encounters scattering, and becomes quasi-ballistic in nature. For considering these effects, we use a projection factor to evaluate our MOSFET drain current as [3], [4] follows:

ID = × ID,Bal. (7) The value of is determined as follows:

= λmax LCh + λmax (8)

where LCh is the channel length and λmax is the mean free path calculated as [3], [4] follows:

λmax = (2ϕT h) 3/2

qμ

F0(ηS − EC) F−1/2(ηS − EC ) (9)

where EC is the top of the conduction band energy in the channel, which is evaluated from the maxima of the self- consistent poten

*View more*